Create Presentation
Download Presentation

Download Presentation
## Effect of Symmetry on the Orientation Distribution

- - - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - - -

**Effect of Symmetry on the Orientation Distribution**27-750 Texture, Microstructure & Anisotropy A.D. Rollett Last revised:28th Mar. ‘14**Objectives**• How to convert Euler angles to an orientation matrix, and back. • Review of symmetry for both crystals and materials processing. • Explain symmetry operators, their matrix representation, and how to use them to find all the symmetrically equivalent descriptions of a given texture component. • To illustrate the effect of crystal and sample symmetry on the Euler space required for unique representation of orientations. • To point out that sample symmetry is statistical rather than physical. Also that orientations related by sample symmetry are, in general, physically distinct. • To explain why Euler space is generally represented with each angle in the range 0-90°, instead of the most general case of 0-360° for 1 and 2, and 0-180° for . • To point out the special circumstance of cubic crystal symmetry, combined with orthorhombic sample symmetry, and the presence of 3 equivalent points in the 90x90x90° “box” or “reduced space”. • To explain the concept of “fundamental zone”. • Part 1 of the lecture provides a qualitative description of symmetry and its effects. Part 2 provides the quantitative description of how to express symmetry operations as rotation matrices and apply them to orientations.**In Class Questions: 1**• What is a fundamental zone? • What is the difference between “crystal symmetry” and “sample symmetry”? • Which kind of symmetry is physical in nature, and which one is statistical? • Which point group is applicable to cubic metals? Hexagonal metals? Tetragonal tin? • List the common types of sample symmetry.**In Class Questions: 2**• What limits on the Euler angles are appropriate to cubic-monoclinic symmetry? • Give an example of a symmetry operator in the hexagonal group 622. • Explain how to start with a set of Euler angles, apply symmetry and obtain a new set of Euler angles for the symmetrically equivalent orientation. • If we apply the symmetry of a given point group, by what factor is the volume of the resulting sub-space decreased, compared to the original orientation volume? • Based on a matrix representation of orientations, do we left-multiply or right-multiply to apply a sample symmetry operator?**In Class Questions: 3**• How can we test our scheme to calculate symmetry-related orientations to make sure that we apply crystal and sample symmetry correctly? • If we change the sample symmetry to monoclinic, how large a space should we use in Euler angle space? • If we change the crystal symmetry to hexagonal, how does this change the range of Euler angles required? Can you explain why the 3rd Euler angle only needs to have the range 0-60°? • Draw a stereographic projection and add ovals to represent diads, triangles to represent triads and squares to represent tetrads until you have a diagram of the O(432) point group.**Geometry of {hkl}<uvw>**Sample to Crystal (primed) ^ ^ Miller indexnotation oftexture componentspecifies directioncosines of crystaldirections // tosample axes. Form the second axis from the cross-product of the 3rd and 1st axes. e’3 e3 // (hkl) [001] [010] ^ e’2 ^ ^ e2 // t ^ e1 // [uvw] ^ e’1 t = hklxuvw [100] Obj/notation AxisTransformation Matrix EulerAngles Components**Form matrix from Miller Indices**Basic idea: we can construct the complete rotation matrix from two known, easy to determine columns of the matrix. Knowing that we have columns rather than rows is a consequence of the sense of rotation, which is equivalent to the direction in which the axis transformation is carried out. Obj/notation AxisTransformationMatrixEulerAngles Components**Bunge Euler angles to Matrix**Basic idea: construct the complete orientation matrix from individual, easy to understand rotations that are based on the three different Euler angles. Demonstrate the equivalence between the rotation matrix constructed from these rotations, and the matrix derived from direction cosines. “Rotation” in this context means “transformation of axes”. Rotation 1 (f1): rotate axes (anticlockwise) about the (sample) 3 [ND] axis;Z1. Rotation 2 (F): rotate axes (anticlockwise) about the (rotated) 1 axis [100] axis;X. Rotation 3 (f2): rotate axes (anticlockwise) about the (crystal) 3 [001] axis;Z2. Obj/notation AxisTransformationMatrixEulerAngles Components**Bunge Euler angles to Matrix, contd.**Combine the 3 rotations via matrix multiplication; 1st on the right, last on the left: A=Z2XZ1 Obj/notation AxisTransformationMatrixEulerAngles Components**Matrix with Bunge Angles**A = Z2XZ1 = [uvw] (hkl) Obj/notation AxisTransformationMatrixEulerAngles Components**Matrix, Miller Indices**• The general Rotation Matrix, a, can be represented as in the following: • Here the Rows are the direction cosines for the 3 crystal axes, [100], [010], and [001] expressed in the sample coordinate system (pole figure). [100]xtaldirection [010]xtaldirection [001]xtaldirection Obj/notation AxisTransformationMatrixEulerAngles Components**Matrix, Miller Indices**• The columns represent components of three other unit vectors: TD ND(hkl) [uvw]RD • Here the Columns are the direction cosines (i.e. hkl or uvw) for the sample axes, RD, TD and Normal directions expressed in the crystal coordinate system. Compare to inverse pole figures. Obj/notation AxisTransformationMatrixEulerAngles Components**Compare Matrices**[uvw] (hkl) [uvw] (hkl) ≡ Basic idea: the complete orientation matrix that describes an orientation must be numerically the same, coefficient by coefficient, regardless of whether it is constructed from the Euler angles, or from the Miller indices. Therefore we can equate the two matrix descriptions, entry by entry. Obj/notation AxisTransformationMatrixEulerAngles Components**Miller indices from Euler angle matrix**Compare the matrix formed from the Miller indices with the Euler angle matrix. Extract indices from the 1st and 3rd columns n, n’ = arbitrary factors to make integers from real numbers Obj/notation AxisTransformation Matrix EulerAngles Components**Euler angles from Orientation Matrix**Notes: the range of inverse cosine (ACOS) is 0-π, which is sufficient for ;from this, sin() can be obtained. The range of inverse tangent is 0-2π, so numerically one must use the ATAN2(y,x) function) to calculate 1 and 2. Caution: in Excel, one has ATAN2(x,y), which is the reverse order of arguments compared to the usual ATAN2(y,x) in Fortran, C (use ‘double atan2 ( double y, double x ); ‘) etc.! Also, if the second Euler angle is too close to zero, then the standard formulae fail because sine() approaches zero (see next slide). The second formula deals with this special case, where the 1st and 3rd angles are linearly dependent; distributing the rotation between them is arbitrary. Corrected -a32 in formula for 1 18th Feb. 05; corrected a33=1 case 13th Jan08**Special Case: = 0**A = Z2IZ1 = Set I is the Identity matrix Obj/notation AxisTransformationMatrixEulerAngles Components**Crystal vs. Sample Symmetry**• An understanding of the role of symmetry is essential in texture. • Two separate and distinct forms of symmetry are relevant: • CRYSTAL symmetry • SAMPLE symmetry • Crystal symmetry is always present (even if, in principle, heavily defected crystals may exhibit lower symmetry) and must always be accounted for. Sample symmetryis only present on a statistical basis, i.e. only a polycrystal can exhibit sample symmetry for the texture as a whole. • Typical usage lists the combination crystal-sample symmetry in that order, e.g. cubic-orthorhombic.**Take-Home Message**The essential points of this lecture are: • Crystal symmetry means that a crystal can be rotated in various ways that leave it unchanged (physically indistinguishable). In orientation space, the equivalent result is that any given orientation is related to exactly as many other orientations as there are symmetry operators (understandable in terms of group theory). • Because there are multiple equivalent points, we usually divide up the full orientation space (e.g. 360°x180°x360° in Euler space) and use only a small portion of it (e.g. 90°x90°x90°). • Sample symmetry has the same sort of effect as crystal symmetry, even though it is a statistical symmetry (and orientations related by a sample symmetry element are physically distinguishable and do have a misorientation between them. Sample symmetry is evident in pole figures whereas crystal symmetry is evident in inverse pole figures. • Unfortunately, Euler space (spherical angles) means that the dividing planes have odd shapes and so for the common cubic-orthorhombic combination, we have 3 copies of the fundamental zone in the range 0-90° for each angle. Rodrigues space is far simpler in this respect because symmetry operators always lead to flat dividing planes.**Deformation vs. Sample Symmetry**• Note that the texture of a material is a consequence of its thermomechanical history (and therefore offers clues about that history). • The (statistical) sample symmetry is directly related to the symmetry of the preceding deformation. • In general, the sample symmetry reflects the lowest symmetry deformation that was imposed on the material. • Rolling is a plane strain deformation, with orthorhombic symmetry. We call it “plane strain” because (in the ideal case) all the strain occurs in one plane, the RD-ND plane with zero strain in the TD (parallel to the axes of the rolls). Torsion is a simple shear, with monoclinic symmetry. Wire drawing is an axi-symmetric deformation with cylindrical symmetry. Upsetting or uniaxial compression is also an axi-symmetric deformation with cylindrical symmetry. Rolling: anvilfire.com torsion: ejsong.com**Pole Figure for Wire Texture**{111} • (111) pole figure showing a maximum intensity at a specific angle from a particular direction in the sample, and showing an infinite rotational symmetry (C). • F.A.=Fiber Axis (parallel to the length of the wire) • A particular crystal direction in all crystals is aligned with this fiber axis (i.e. a particular sample direction). • For a cubic material, this combination would be classed as cubic-cylindrical. forth-armoury.com In this case, <100> // F.A.**Effect of Symmetry**• Illustration of 3-fold, 4-fold, 6-fold rotational symmetry The essential point about applying a symmetry operation is that, once it has been done, you cannot tell that anything has changed. In other words, the rotated or reflected object is physically indistinguishable from what you started with. Note the symbols used to denote the different rotational symmetry elements.**Effect of Symmetry: Example**• Note how one can re-label the axes but leave the physical object (crystal) unchanged. • Which symmetry operator was applied (from O(432))? [001] [100] [010] [010] [001] [100]**Stereographic projectionsof symmetry elements and general**poles in thecubic point groupswith Hermann-Mauguinand Schoenfliesdesignations. Note the presence of four triad symmetry elements in all these groups on <111>. Cubic metals mostlyfall under . Groups: mathematical concept, very useful for symmetry**Sample Symmetry**Torsion, shear:Monoclinic, 2. Rolling, plane straincompression, mmm. Otherwise,triclinic. Axisymmetric: C**Fundamental Zone**• The fundamental zone (or asymmetric unit) is the portion or subset of orientation space within which each orientation (or misorientation, when we later discuss grain boundaries) is described by a single, unique point. • The fundamental zone is the minimum amount of orientation space required to describe all orientations. • Example: the standard stereographic triangle (SST) for directions in cubic crystals. • The size of the fundamental zone depends on the amount of symmetry present in both crystal and sample space. More symmetry smaller fundamental zone. • Note that in Euler space, the 90x90x90° region typically used for cubic [crystal]+orthorhombic [sample] symmetry is not a fundamental zone because it contains 3 copies of the actual zone!**Symmetry Issues**• Crystal symmetry operates in a frame attached to the crystal axes. • Based on the definition of Euler angles, crystal symmetry elements produce relations between the second & third angles. • Sample symmetry operates in a frame attached to the sample axes. • Sample symmetry produces relations between the first & second angles. • The combination of crystal and sample symmetry is written as crystal-sample, e.g. cubic-orthorhombic, or hexagonal-triclinic.**Choice of Section Size**• Quad, Diad symmetry elements are easy to incorporate, but Triads are highly inconvenient. • Four-fold rotation elements (and mirrors in the orthorhombic group) are used to limit the third, f2, (first, f1) angle range to 0-90°. • Second angle, F, has range 0-90° (diffraction adds a center of symmetry).**Section SizesCrystal - Sample**• Cubic-Orthorhombic: 0f1 90°, 0F90°, 0f2 90° • Cubic-Monoclinic: 0f1 180°, 0F90°, 0f2 90° • Cubic-Triclinic: 0f1 360°, 0F90°, 0f2 90° • But, these limits do not delineate a fundamental zone.**f2**Points related by triad symmetryelement on <111>(triclinicsample symmetry) F f1 Take a point, e.g. “B”; operate on it with the 3-fold rotation axis (blue triad); the set of points related by the triad are B, B’, B’’, with B’’’ being the same point as B. The point is, that as you operate on a point (orientation) with a symmetry operation, in general all the Euler angles change. [Bunge]**Effect of 3-fold axis**section in f1 cuts through more than one subspace Regions I, II and III are related by the triad crystal symmetry element, i.e. 120° about <111>, combined with sample symmetry. [Bunge]**Example of 3-fold symmetry**The “S” component,{123}<634> has angles {59, 37, 63}also {27,58,18},{53,74,34} and occurs in three related locations in Euler space. 10° scattershown about component. Regions I, II and III are related by the triad crystal symmetry element, i.e. 120° about <111>, combined with sample symmetry. [Randle & Engler, fig. 5.7]**S component in f2 sections**Regions I, II and III are related by the triad symmetry element, i.e. 120° about <111>. 10° scattershown about the S component. Randle & Engler, fig. 5.7**Orthorhombic Sample Symmetry (mmm) Relationships in Euler**Space f1=0° 360° 180° 270° 90° diad F ‘mirror’ ‘mirror’ = 180° 2-fold screw axis changes f2by π Note: this slide illustrates how the set of 3 diads (+ identity) in sample space operate on a given point. The relationship labeled as ‘mirror’ is really a diad that acts like a 2-fold screw axis in Euler space.**Sample symmetry, detail**Tables for Texture Analysis of Cubic Crystals, Springer Verlag, 1978**Crystal Symmetry Relationships (432) in Euler Space**3-fold axis 360° 180° 270° 90° f2=0° F 4-fold axis Other 4-fold, 2-fold axis:act on f1 also = 180° Note: points related by triad (3-fold) have different f1 values.**Crystal symmetry: detail**Tables for Texture Analysis of Cubic Crystals, Springer Verlag, 1978**How many equivalent points?**• For cubic-orthorhombic crystal+sample symmetry, we use a range 90°x90°x90° for the three angles, giving a volume of 90°2 (or π2/4 in radians). • In the (reduced) space there are 3 equivalent points for each orientation (texture component). Both sample and crystal symmetries must be combined together to find these sets. • If we look within the full orientation space then there are as many equivalent points as there are symmetry elements. Thus for cubic crystal symmetry there are 24 equivalent points; for hexagonal 12 etc. • Fewer (e.g. Copper) or more (e.g. cube) equivalent points for each component are found in the reduced spaceif the the component coincides with one of the symmetry elements.**Volume of Orientation Space**• O(432) has 24 operators (i.e. order=24); O(222) has 4 operators (i.e. order=4): why not divide the volume of Euler space (8π2, or, 360°x180°x360°) by 24x4=96 to get π2/12 (or, 90°x30°x90°)? • Answer: we leave out a triad axis (because of the awkward shapes that it would give us), so we divide by 8x4=32 to get π2/4 (90°x90°x90°). • This is an illustration of group theory in action. Each set of symmetry operators divides up the orientation space by a factor equal to the number of elements in the group. • The reason is, essentially, a question of counting: each point in one zone has exactly one point in another zone related by a given operator.**Group theory approach**• Again, this is an illustration of group theory in action. Each set of symmetry operators divides up the orientation space by a factor equal to the number of elements in the group. • Crystal symmetry:a combination of 4- and 2-fold crystal axes (2x4=8 elements) reduce the range of Ffrom π to π/2, and f2 from 2π to π/2. • Sample symmetry:the 2-fold sample axes (4 elements in the group) reduce the range of f1 from 2π to π/2. • Volume of {0 f1, F, f2 π/2} is π2/4. • The reason is, essentially, a question of counting: each point in one zone has exactly one point in another zone related by a given operator.**Special Points, Partial Fibers**No. of points in the 90x90x90° space Copper: 2 Brass: 3 S: 3 Goss: 3 Cube: 8 Dillamore: 2 Why this variation?Points that fall on the edge may appear more, or fewer times than the standard count of 3. Humphreys & Hatherly**Sample Symmetry Relationships in Euler Space: special points**f1=0° 360° 180° 270° 90° diad F diad diad = 90° Cube lies on the corners Copper, Brass, Goss lie on an edge, so that they coincide with a symmetry element**3D Views**a) Brass b) Copper c) S d) Goss e) Cube f) combined texture 1:{35, 45, 90}, Brass, 2:{55, 90, 45}, Brass 3:{90, 35, 45}, Copper, 4:{39, 66,27}, Copper 5:{59, 37,63}, S, 6:{27, 58,18}, S, 7:{53, 75,34}, S 8:{90, 90, 45}, Goss9: {0, 0, 0}, cube*10:{45, 0, 0}, rotated cube * Note that the cube exists as a line between (0,0,90) and (90,0,0) because of the linear dependence of the 1st and 3rd angles when the 2nd angle = 0. Figure courtesy of Jae-hyung Cho**Special Points: Explanations**• Points coincident with symmetry axes may also have equivalent points, often on the edge. Cube: should be a single point, but each corner is equivalent and visible. • Goss, Brass: a single point becomes 3 because it is on the f2=0 plane. • Copper: 2 points because one point remains in the interior but another occurs on a face; also the Dillamore orientation. • Note for later about volume fractions: although the volumes enclosed by the 12° capture (misorientation) distance shown in the figure vary with the 2nd euler angle, to first order it is the symmetry planes that control the volume fractions. So S, for example, has 3 complete “blobs” whereas Goss has only 3 x ¼ and so will contain only ~1/4 of the volume fraction of S, based on a random (uniform) texture.**Meaning of “Variants”**• The existence of variants of a given texture component is a consequence of (statistical) sample symmetry. • If one permutes the Miller indices for a given component (for cubics, one can change the sign and order, but not the set of digits), then different values of the Euler angles are found for each permutation. • If a pole figure is plotted of all the variants, one observes a number of physically distinct orientations, which are related to each other by symmetry operators (diads, typically) fixed in the sample frame of reference. • Each physically distinct orientation is a “variant”. The number of variants listed depends on the choice of size of Euler space (typically 90x90x90°) and the alignment of the component with respect to the sample symmetry.**Part 2: Quantitative**• In part 2 of the lecture, we describe the methods for describing symmetry operations as rotation matrices and how to apply them to texture components, also expressed as matrices. • Notation:orientation: g(crystal) symmetry operator: OC(sample) symmetry operator: OS**Rotations: definitions**• Rotational symmetry elements exist whenever you can rotate a physical object and result is indistinguishable from what you started out with. • Rotations can be expressed in a simple mathematical form as unimodularmatrices (or, orthogonal matrices), often with elements that are usually either one or zero (but not always!). • When represented as matrices, the inverse of a rotation is equal to the transpose of the matrix. • Rotations are transformations of the first kind; determinant = +1. • Reflections (not needed here) are transformations of the second kind; determinant = -1. • Crystal symmetry also can involve translations but these are not included in this treatment.**Rotation Matrixfrom Axis-Angle Pair**Written out as a complete 3x3 matrix:**Symmetry Operator examples**• Diad on z: [uvw] = [001], = 180° - substitute the values of uvw and angle into the formula • 4-fold on x: [uvw] = [100] = 90°**-**Matrixrepresentation of the rotation point groups What is a group? A group is a set of objects that form a closed set: if you combine any two of them together, the result is simply a different member of that same group of objects. Rotations in a given point group form closed sets - try it for yourself! Note:the 3rd matrix in the 1st column (x-diad) is missing a “-” on the 33 element; this is corrected in this slide. Also, in the 2nd from the bottom, last column: the 33 element should be +1, not -1. In some versions of the book, in the last matrix (bottom right corner) the 33 element is incorrectly given as -1; here the +1 is correct. Kocks, Tomé, Wenk:Ch. 1 Table II The 4 operators enclosed in orange boxes are also the 222 point group, appropriate to orthorhombic symmetry